Lanthanide Thioborates, an Emerging Class of Nonlinear Optical Materials, Efficiently Synthesized Using the Boron-Chalcogen Mixture Method
Breton, Logan S.; Morrison, Gregory; Lacroix, Matthew; Halasyamani, P. Shiv; Zur Loye, Hans-Conrad; Chemical Communications  (2022) –; doi:10.1039/D2CC01260J

data_7130258
_publ_section_title
;
 Lanthanide Thioborates, an Emerging Class of Nonlinear Optical Materials,
 Efficiently Synthesized Using the Boron-Chalcogen Mixture Method
;
_journal_name_full               'Chemical Communications'
_journal_paper_doi               10.1039/D2CC01260J
_journal_year                    2022
_chemical_formula_moiety         'B Ce S3'
_chemical_formula_sum            'B Ce S3'
_chemical_formula_weight         247.11
_chemical_name_systematic        'Cerium Orthothioborate'
_space_group_crystal_system      orthorhombic
_space_group_IT_number           33
_space_group_name_Hall           'P 2c -2n'
_space_group_name_H-M_alt        'P n a 21'
_atom_sites_solution_primary     direct
_audit_creation_date             2022-01-25
_audit_creation_method
;
Olex2 1.3
(compiled 2020.11.12 svn.r5f609507 for OlexSys, GUI svn.r6408)
;
_audit_update_record
;
2022-02-25 deposited with the CCDC.	2022-06-20 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.6059(2)
_cell_length_b                   6.01810(10)
_cell_length_c                   8.9311(2)
_cell_measurement_reflns_used    9850
_cell_measurement_temperature    300.8
_cell_measurement_theta_max      36.30
_cell_measurement_theta_min      3.52
_cell_volume                     408.804(16)
_computing_cell_refinement       'SAINT V8.40B (?, 2016)'
_computing_data_reduction        'SAINT V8.40B (?, 2016)'
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXS  (Sheldrick, 2008)'
_diffrn_ambient_temperature      300.8
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0357
_diffrn_reflns_av_unetI/netI     0.0117
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            44388
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         36.323
_diffrn_reflns_theta_min         4.083
_diffrn_source_current           1.4
_diffrn_source_power             0.07
_diffrn_source_voltage           50.0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    12.429
_exptl_absorpt_correction_T_max  0.2740
_exptl_absorpt_correction_T_min  0.1586
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016) was used for absorption correction.
wR2(int) was 0.1190 before and 0.0527 after correction.
The Ratio of minimum to maximum transmission is 0.5788.
The \l/2 correction factor is Not present.
;
_exptl_crystal_colour            green
_exptl_crystal_colour_primary    green
_exptl_crystal_density_diffrn    4.015
_exptl_crystal_description       rod
_exptl_crystal_F_000             444
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.492
_refine_diff_density_min         -0.289
_refine_diff_density_rms         0.074
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.335(10)
_refine_ls_extinction_coef       0.0057(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.124
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     48
_refine_ls_number_reflns         1970
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.124
_refine_ls_R_factor_all          0.0080
_refine_ls_R_factor_gt           0.0079
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0052P)^2^+0.0702P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0173
_refine_ls_wR_factor_ref         0.0174
_reflns_Friedel_coverage         0.903
_reflns_Friedel_fraction_full    0.997
_reflns_Friedel_fraction_max     0.999
_reflns_number_gt                1960
_reflns_number_total             1970
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d2cc01260j2.cif
_cod_data_source_block           lb2059c_pt2_os
_cod_database_code               7130258
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_max   0.707
_shelx_estimated_absorpt_t_min   0.477
_olex2_refinement_description
;
1. Twinned data refinement
 Scales: 0.665(10)
 0.335(10)
;
_shelx_res_checksum              12330
_shelx_hkl_checksum              38639
_olex2_submission_special_instructions 'No special instructions were received'